from materials modelling to
Faculdade de Cicncias e Tecnologia da
International Federation for Structural
Universidade de Coimbra
"Fire Design of Concrete Structures
-From Materials Modelling to Structural Performance"
Proceedings of the International
"Fire Design of Concrete Structures
-From Materials Modelling to Structural Performance"
University of Coimbra
Coimbra - Portugal
Joao Paulo Correia Rodrigues
Department of Civil Engineering Faculty of Sciences and Technology
University of Coimbra Coimbra, Portugal
Gabriel Alexander Khoury
Department of Civil Engineering Imperial College London, UK
Padua University, Italy
Proceedings of the International Workshop
"Fire Design of Concrete Structures - From Materials Modelling to
2008 Joao Paulo Correia Rodrigues, Gabriel Alexander Khoury and
Joao Paulo Correia Rodrigues
Gabriel Alexander Khoury
No part of this work may be reproduced, stored in a retrieval system, or transmitted in any
fonn or by any means, electronic, mechanical, photocopying, microfilming, recording or
otherwise, without written pennission from the Publisher, with the exception of any material
supplied specifically for the purpose of being entered and executed on a computer system, for exclusive use by the purchaser of the work.
Department of Civil Engineering, Faculty of Sciences and Technology, Universidade de Coimbra - Polo II,
Rua Luis Reis Santos,
Improvements in structural ftre safety have significant positive implications to life-time costs
and human safety records of concrete structures. For this reason the subject has been, for a long
time, of high interest amongst researchers, academics and practicing engineers as well as users,
owners and the authorities. The subject is challenging especially because of the complex
nature, and behaviour, of concrete as a material during fIre and because of the nature of ftre
itself which could involve rapid heating to 800-1000'C or more. This subject is by no means fully investigated and there is a need for a bettcr understanding of the response of concrete materials and structures to the thermal shock that fire presents - leading to improved designs intended to combat this ever-present potential problem.
The authors contributing to this workshop came from various parts of the world. Some individuals and organisations are leading experts in the field for many years if not decades. The synergy between the different complimentary subjects and different experts provides a valuable up-ta-date compilation, and insight, encompassed within these proceedings. There were 54 papers presented at the workshop falling under a comprehensive array of complimentary topics
such as: (1) Physical and mechanical properties for fire design; (2) Micro-structural modelling;
(3) Spalling; (4) Sectional analysis and structural behaviour; (5) Influence of materials behaviour on structural performance; (6) Detailing and connections; (7) Assessment and repair afler fire; (9) Real fires, large-scale tests and model validation.
The purpose of such a workshop is not only to bring people together with a common purpose but also to inspire the workshop participants and readers of these proceedings with new ideas, methodologies and discoveries critical to the promotion of improved structural fire safety design. This workshop indeed presents new insights and developments which are too many to
li st in this forward. They include the development of a new NMR technique that measures
non-intrusively the moisture content of cement pastes down to below the levels measured
intrusively by mercnry porosimetry and Nitrogen intrusion. The development of new optical equipment for the assessment of fire damaged concrete structures. A new understanding of how polypropylene fibres contribute to pore pressure reduction in fire and hence the reduction in the risk of explosive spalling. Impressive developments in numerical structural fire modelling which are integrated with advances in materials testing and knowledge. A note of caution for
incoming researchers is to be critical when reading the literature, to conserve energies and
resources in future research by investigating some of the many areas that still require
development, and by clearing out confusions in terminology.
The 2-day Coimbra fib Workshop on "Fire Design of Concrete Structures - From Materials Modelling to Structural Performance" was held at Coimbra University (portugal) on the 8th and 9th of November 2007 and follows close on the heel of the completion of the fib State-of-the-art report bulletin 38 on "Fire Design of concrete structures - materials, structures and modelling" published in April 2007. The conference was attended by 93 participants from 21
different countries among which many young researchers.
Gabriel Alexander Khoury (Convener fib WP 4.3.1)
Niels Peter Hoj (Convener fib TO 4.3)
• Joao Paulo
Univ. Coimbra - Portugal
• Luc Taerwe (Co - Chairman) - (Convener
Ghent University - Belgium
• Niels Peter Hoj (Convener
HOJ Consulting GmbH - Switzerland
• Gabriel Alexander Khoury (Convener
Imperial College London - UK
• Pietro G. Gambarova
Politecnico di Milano - Italy
• Alberto Meda
University of Bergamo - Italy
• Fernando Jose F. Branco
University of Coimbra - Portugal
• Aldina Maria C. Santiago
University of Coimbra - Portugal
• Alberto Meda - University of Bergamo - Italy • Angel Arteaga - Instituto Eduardo Torroja - Spain
• Antonio Le~a Coelho - LNEC - Portugal
• Arnold Van Acker - Belgium
• Arnoud Breunese - TNO - The Netherlands • Carmello Majorana - University of Padua - Italy • Ekkehard Richter - Tech_ Univ_ of Braunschweig - Germany
• Fabienne Robert - CERIB - France
• Gabriel Alexander Khoury - Imperial College London - UK • Jean-Claude Dotreppe - University of Liege - Belgium
• Jean-Fran~ois DenoiH - FEBELCEM - Belgium • Jean-Marc Franssen- University of Liege - Belgium
• Jesus Rohena - FHWA - USA
• Joao Paulo Co Rodrigues - University of Coimbra - Portugal
• Joaquim Barros - University of Minho - Portugal
• Jose Maria Izquierdo - Intemac - Spain
• Josko Ozbolt- University of Stuttgart - Germany • Kese Both - TNO - The Netherlands
• Long Ph an - NIST - USA
• Luc Taerwe - Ghent University - Belgium • Mamoud Behloul - Lafarge - France • Paolo Riva - University of Brescia - Italy • Patrick Bamonte - Politecnico di Milano - Italy • Pietro Gambarova- Politecnico di Milano - Italy • Roberto Felicetti - Politecnico di Milano - Italy • Sergio Lopes - University of Coimbra - Portugal
• Steward Matthews - BRE - UK • Tom Lennon - BRE- UK • Ulla-Maija Jumppanen - Finland
• Ulrich Diederichs - University of Rostock - Germany • Xianyu Jin - Zhejiang University- China • Yngve Anderberg - Fire Safety Design AB - Sweden
• Yoshikazu Ota - Ota Engineering - Japan
TABLE OF CONTENTS
FOREWORD ... . ... ... .... .. .. ... . .. . ... ... •.. . ... . .. . ... ....•... . ... ... V
COMMITIEES .. ... ... . ... ... . ... ... . .. ... ... ... VII
SPONSORS ... .. ... . ... . .. .. ... . .. . ... ... . .. . ... . ... . .. . ... .IX
TABLE OF CONTENTS ... .. ... .. ... . ... XI
AUTHOR INDEX ... .. ... .. ... .. .. .. ... ... .595
SESSION I - PHYSICAL AND MECHANICAL PROPERTIES FOR FIRE DESIGN
...••...••••... ...•••...•...•...•... 1
• Fire and concrete: from materials behaviour to application
Gabriel Alexander KHOURY
... ... 3
• Experimental study of mechanical behaviour of high performance concrete at high temperature
Jean-Christophe MINDEGUIA, Pierre PIMIENTA, Arnaud BEUROTTE, Christian BORDERIE and Helene CARRE
... . ... 25
• Experimental investigations concerning high temperature behaviour of ultra high
Ulrich DIEDERICHS and Vesa PENTTALA
• Compression tests of high-strength concrete cylinders at elevated temperature
Takeo HIRASHIMA, Koji TOYODA, Heisuke YAMASHITA , Masatoshi TOKOYODA and Hideki UESUGJ
... . .... ... .47
• High-temperature resistance and thermal properties of self-compacting concrete: preliminary results
Patrick BAMONTE and Pietro G. GAMBAROVA
• Dehydration and rehydration processes in cementitious materials after fire. Correlation between micro and macrostructural transformations
Cruz ALONSO and Lorenzo F. MUNICIO
... ... .. ... ... .. ... ... ... .. ... 69
SESSION 2 - MICRO - STRUCTURAL MODELLING
... ... ... .... .. ... ... ... .. ... .... .. .. .. ... .... ... . ... . 79
• Micro-structural modelUng of concrete under fire conditions
Carmelo E. MAJORANA, Valentina A. SALOMONl and Gabriel Alexander KHOURY
... ... . . ... ... .... ... .... .. ... ... 81
• Towards prediction of the thermal spalling risk through a multi-phase porous media
model of concrete
Francesco PES A VENTO, Bernhard SCHREFLER, Carmelo MAIORANA and Dariusz GA WIN
... ... ... .. ... .. ... .. .. ... ... . ... ... . . .. .. .. .. .... ... 95
• An experimental study of transient strain for a concrete with limestone aggregate
Masatoshi TOKOYODA, Heisuke YAMASHITA, Koji TOYODA, Takeo HIRASHIMA, and Hideki UESUGI
... ... ... .. ... .... . ... . ... 105
• A model for the structural behaviour of bored tunnels during fire
B.B.G. LOTTMAN, E.A.B. KOENDERS , C.B.M. BLOM and V. BOUWMAN
.... .. .. ... . .. ... ... ... . ... ... ... . ... .. ... 115
• Modelling localised failure of reinforced concrete slabs in fire
Xinmeng YU , Zhaohui HUANG, Ian BURGESS and Roger PLANK
... ... ... .. ... ... ... .... .. .. .. ... ... ... ... 127
• Damage and strength reduction of a high performance concrete due to thermomecbanical stresses
Sven HUISMANN , Joao Paulo C. RODIUGUES and Manfred KORZEN
... . . ... ... . ... . .. ... ... .... ... . ... ... ... . ... ... 141
• Assessment of the equivalent thermal diffusivity for fire analysis of concrete structures
Roberto FELIC ETTI
... . .. ... . .... .... ... .... ... . ... ... ... ... . ... 149
SESSION 3 - SPALLING
... ... . ... .. ... . ... . .. .. ... ... .... . . . .... ... 159
• Explosive spalling of concrete under fire conditions
Ulrich SCHNEIDER and Johannes HORVATH
... ... .. ... ... ... ... .. ... 161
• Experimental study of the influence of polypropylene fibres on material properties and
fire spalling of concrete
Robert JANSSON and Lars BOSTROM
... ... ... ... ... ... ... .... ... .. ... . ... .... . ... ... .... ... .. .. .. ... .. 177
• Explosive spalling mitigation mechanism of fiber reinforced high strength concrete
under high temperature condition
Sofren SUHAENDI and Takashi HORIGUCHI
• Effects of spalling on the behaviour of reinforced concrete structures in fire
Zhaohui HUANG, Ian W. BURGESS and Roger J. PLANK
• Polypropylene fibres and explosive spalling
Gabriel Alexander, KHOURY and Carmela E. MAIORANA
... . ... 211
• Experimental study of fire behaviour of different concretes - thermo-hydral and
Jean-Christophe MINDEGUIA, Pierre PIMJENTA, Christian La BORDERIE and Helene CARRE
• Numerical analysis of spalling of concrete cover at high temperature
Josko O:lBOLT, Goran PERISKIC and Hans-Wolf REINHARDT
... . ... . ... 237
SESSION 4 - SECTIONAL ANALYSIS AND STRUCTURAL BEHAVIOUR
... ... 251
• From member design to global structural behaviour
• Nonlinear analysis of shallow parabolic concrete arches under thermal loading Mark A. BRADFORD and R. Ian GILBERT
• Ultimate bending moment capacity of reinforced concrete beam sections at high temperatures
Miguel GON<;;ALVES and Joao Paulo C. RODRIGUES
... " .. . ... . ... 281
• Analytical safety assessment of RC frames exposed to fire naria VENANZI and Marco BRECCOLOTTI
• The buckling of slender concrete and concrete filled columns in fire
Shan-Shan HUANG, Ian BURGESS, Zhao-Hui HUANG and Roger PLANK
• Layered section analysis of RC slabs subjected to fire
Darius BACINSKAS, Gintaris KAKLAUSKAS and Viktor GRIBNIAK
• Plastic-hinge approach for performance-based assessment of RC columns under fire Alexandre LANDESMANN, Daniel MOUCO and Joao Paulo C. RODRIGUES
SESSION 5 - INFLUENCE OF MATERIAL BERA VIOUR ON STRUCTURAL
... ... ... ... ... . ... .. .. .... ... ... ... ... ... 325
• Macroscopic finite element model for tracing the response of concrete structures under fire conditions
Venkatesh KODUR, Monther DW AJKAT and Nikhil RAUT
• Study on fracture toughness of hybrid fiber reinforced high-strength concrete at higb
Takashi HORIGUCHI, Kazoo WATANABE and Soften Leo SUHAENDI
... .. ... .... ... .. ... ... .... .... .... . 343
• Temperature and shear capacity calculation for prestressed hollow core slabs under fire conditions
Yahi. MSAAD and Aodre CHEFDEBIEN
... ... . . .. ... .. ... . .. ... 351
• Numerical evaluation of the fire behaviour ofa concrete tunnel integrating the effects of spalling
Jean -Mark. FRANSSEN, F. HANUS and J.-C . DOTREPPE
• On the effects of structural stability on the M-N envelopes of thermally-damaged RC sections
... .... ... ... ... . ... ... 369
• A new risk-based approach to predict spalling of ordinary strength concrete walls subjected to fire
Susan LAMONT, Barbara LANE, Rachel YIN, Alexander HEISE and Linus LIM
• Influence of ageing on the higb temperature behaviour of cemcntitiollS materials
Frank DEHN and Klaus PISTOL
... .. ... ... ... ... ... ... .... ... ... 393
• Comparison of an approximated method with FEA calculations for the evaluation of
the fire resistance of concrete tunnel sections
Ulrich SCHNEIDER, Martin SCHNEIDER and Jean-Marc FRANSSEN
... ... ... ... ... ... ... ... ... ... •...•... .401
SESSION 6 - DETAILING AND CONNECTIONS
• Current research needs for the fire design of precast concrete building structures in
U. S. practice
• Behaviour of a fibre reinforced concrete tunnel segment submitted to fire
Adorito ALVES, Joao Paulo C. RODRlGUES, Joaquim BARROS, Lucio LOUREN<;O and Simao SANTOS
• Effect of the end and side connections to the hollowcore concrete flooring systems in fire
Jeremy CHANG, Andrew H. BUCHANAN, Rajesh P. DHAKAL and Peter J. MOSS ... ... ... ... .. .... ... .437
• Influence of the temperature on the strength of single adhesive anchors under tensile load
Fernando G. BRANCO, Maria de Lurdes BELGAS and Antonio TADEU
• Push-out tests for partially encased beams at elevated temperature
Paulo A. G. PILaTO, Ana B. Ramos GA VILAN, Luis M. R. MESQUITA and Luisa BARREIRA
• Effects of elevated temperatures on properties concrete blocks
Brian HARDIE, Ali NADJAI and Faris ALI
SESSION 7 - ASSESSMENT AND REPAffi AFTER FIRE
... ... .. ... ... ... . ... .481
• Recent advances and research needs in the assessment of fire damaged concrete
... .... ... 483
• Approaches for the assessment of the residual strength of concrete exposed to fire
Emmanuel ANNEREL and Luc TAERWE
• Repair of fire damaged RC beams with high performance fiber reinforced concrete
Alberto MEDA and Zila RlNALDI
... ... ... .. .. .... .... ... . ... 501
• Experimental study on triaxial behaviour of concrete after exposure to high
Teng Hooi TAN and Zhen LI
.... ... ... ... ... .. ... ... ... . .... . ... ... .. .... ... .. 511
• NMR relaxometry measurements on heated cement paste
Gijs van der HEIIDEN, Leo PEl and Henk HUININK
... . . .. ... ... .. ... ... ... .. ... ... ... .... . ... ... ... ... 523
• Estimation of fire damage in high-strength mortar mixed polypropylene fibers by ultrasonic tomography
Sang Jun PARK and Yasuo TANlGAWA
... .... ... .... .. ... . .. . .. ... .. ... 529
SESSION 8 - REAL FIRES, LARGE-SCALE TESTS AND MODEL VALIDATION
... . . ... ... ... ... .. ... ... ... ... .. .... ... . ... .. ... . ... .. .... 539
• The need for large-scale fire tests Tom LENNON
... .. . ... .. ... .. ... ... ... .... . .. ... ... .. ... . ... ... 541
• Overview of fire testing of concrete and concrete protection systems for tunnels in
Maria HJOHLMAN, Lars BOSTROM and Robert JANSSON
... . ... 551
• The Dalmarnock fire tests on a cast in-situ concrete structure
Susan DEENY, Cecilia A. EMPIS, Tim STRATFORD, M. GILLIE and J. L. TORERO
... .. ... .. ... ... ... ... ... 559
• Effects of fire on a concrete structure: modelling the Windsor tower
Ian FLETCHER, Stephen WELCH, Jorge A. CAPOTE, Daniel AL YEAR and Mariano LAzARO
... .. ... ... ... .. ... ... ... ... ... ... 571
• Case study: concrete beam submitted to natural fire
Nicolas T AILLEFER, Anne MULLER, Philippe FROMY and Fran90is DEMOUGE ... . ... . ... . .. ... . ... ... ... .. ... .. ... ... 583
international workshop "Fire Design of Concrete Structures - From Materials Modelling 10
Structural PelformallCe" - University of Coimbra-Porfugal - November 2007
PUSH-OUT TESTS FOR PARTIALLY ENCASED BEAMS AT
Paulo A. G. Piloto" Assistant Professor Polytechnic Institute of Braganya, Portugal.
Ana B. Ramos
Gavilan Assistant Lecturer EPSZ - University of Salamanca, Spain.
Luisa Barrcira Laboratory Technician Polytechnic Institute of Brogan,a. Portugal
Mesquita Assistant Lecturer Polytechnic Institute of Braganya, Portugal.
Keywords: Elevated temperatures, bond strength, partially encased beams, push-out tests.
Partially encased beam is a steel-concrete composite element, made-up with a hot rolled profile and filled with concrete between flanges. Such structural element improves load-bearing capacity at elevated temperature. The mechanical and thermal interaction between steel and concrete is analysed for natural adherence at elevated temperature, using push-out tests to detennine bond stress and thennal capacitance.
Partially encased beam improves load-bearing capacity of steel profile at elevated temperature. Concrete between flanges reduces the heating rate through the steel profile under fire conditions. The condition for natural adherence is considered between steel and concrete. Bond stress should determine the strength limit state during splitting contact, being represented by the maximum shear stress at steel-concrete interface, which enables both materials to acquire composite action, see figure 1 .
• COlTesponding author ~ Department of Applied Mechanics. School of Technology and Management. Polytechnic Institute of Braganya - Campus Santa Apalonia. 5301-857 BragllnY3. Portugal. Telet: +351 273 303157 Fax: +351 273 313051. e-mail: firstname.lastname@example.org
Paulo A. G. Pilolo, Ana B. Ramos Gavilan , Luis M R. Mesquita and Luisa Ban'eira
/ _~ .. /. ·/010·
IrE·IOIl / _,':.t.:.·"":":; -;; n .f' -"· .~ .
3.:::;, . - • :--- . ""--",,
" ... . ' ;. "
I M '7/'~ 777,;
1 _ _
'2 ~ L: 7
Figure I - Model for partially encased beam at elevated temperature.
When concrete is subjected to high temperatures, deterioration of mechanical properties arises and becomes an important factor to account for. Of particular importance is the loss in
compressive strength and the collapse of bond between the cement paste and aggregates and
the overall interface between steel and concrete. As the temperature approaches 250 ["C]
dehydration begins to take place and the compressive strength begins to reduce. At 300 ["C]
strength reduction would be in the range of 15-40 % and at 550 ["C] reduction in compressive
strength would typically range from 55% to 70% of its original value, [I], being this process
Steel also presents mechanical properties degradation, in a different temperature scale.
Temperature between 550 and 650 ["C] is responsible for residual stress cutback, reducing its
elastic modulus and yield stress to 60 % and 78%, respectively at 500 ["C]. Between 500 ["C]
and 700 ['C] these values fall very much and after 700-800 ["C] steel becomes with a new
austenitic phase, responsible for changing thermal and mechanical properties.
This work presents an experimental method for testing mechanical and thermal characteristics
for the interface of partially encased beams at elevated temperature (400 ["C]), which will be valuable for the interface numerical modelling. Interface may be represented by non linear
finite spring element, introducing contact stiffness and conductance.
Push-out test is based on axially load concrete blocks by means of a hydraulic jack, at high
temperature level, measuring the relative displacement of concrete, determining the load
histogram. Load is stepped incremented up to the ultimate state conditions (slipping of
concrete or local concrete failure). A set of three tests were carried out.
2. SPECIMEN PREPARATION
Partially encased beams were prepared in laboratory with S275JR IPE 100 steel profile and low strength reinforced concrete. Reinforcement was attained with 8 [mm] diameter B500s rib bars welded to 4 [mm] plain diameter steel bars for stirrups, spaced every 135 [mm]. The interface
Push-out tests for partially encased beams at elevated temperature
between steel and concrete is made without shear connectors, being natural adherence characterized by chemical and friction characteristics.
Minimum concrete cover shall be provided in order to ensure the safe transmission of bond
forces, the protcction of steel against corrosion (durability) and appropriate fire resistance. An
external vibration and punching should guarantee the best consolidation and consequently the
highest adherence between both materials, see figure 2. Cure was attained inside wet chamber
at 23 ± 1,7"C and at least 95% of relative humidity, during 28 days.
Figure 2 - Specimen preparation.
Every partially encased beam was set up with 650 [rnm]long steel, filled with 540 [rnm]long concrete block. Concrete should fill in between flanges and leave 110 [mm] air gap in the
bottom flanged beam to allow measurement of concrete relative displacement.
Steel surface roughness was characterized according to ISO 4287 / 4288 standards, [2,3], along a specified evaluation length of 12.5 [rnm], with 5 roughness sampling length of 2.5 [rnm] each. Roughness was measured in every tested bearn, each with 18 evaluation lengths. Arithmetic average roughness of 3.22 [flm] was determined which fall in-between expected values for this fmished product (0,8 to 3,2 [flml), . This steel surface condition with concrete should produce a dry friction coefficient between 0.2 and 0.6, .
Specimens from steel profile were cut and normalized. Steel was received from manufacture
with nominal yield stress equal to 490 [MPa], based on 6 tested specimens, with I I [MPa] of standard deviation, .
Portland cement type II class CEM-IIIB-L 32,5 N and siliceous aggregate were used in the
concrete elaboration. Aggregate dimensions were restrained to web flange dimensions and also to volumetric concrete recover dimensions, using an average diameter equal to 4 [mm]. Specimens from concrete were produced and normalized for cubic compressive tests,
accordiog to EN 12390-2, . Compressive strength for hardened concrete at 7 and at 28 days
was determined. The average value of cube compressive strength allows concrete to be
classified as CI2/15. The residual humidity was detennined equal to 6.75%.
Steel reioforcement was also classified according to standard procedures. From the 8 [rnm] rebar B500s samples were, prepared and tested according to standard , resulting yield stress
Paulo A. G. Pi/DID, Ana B. Ramos Gavildn, Luis M R. Mesquita and Luisa Barreiro
equal to 500 [MPa]. Specimens from steel stirrups were produced and normalized for tensile tests, using same standards, resulting yield stress equal to 200 [MPa].
3. EXPERIMENTAL TESTS FOR PUSH-OUT
For testing partially encased beams under elevated temperature, an insulated chamber was
created, using an electro-ceramic device to increase temperature, see figure 3. Low thennal
conductivity materials were applied in insulated chamber, using vermiculite plate and special thermo-resistant glass material.
Figure 3 - Experimental set-up for push-out at elevated temperatures.
A heating rate of 400 ["CIh] was applied up to the specified test temperature level (400 rOC]).
After temperature stabilization, both concrete blocks were mechanically loaded using an incremental force system up to the maximum force level (maximum bond strength). After that, an incremental displacement method was applied to find out the post bond hehaviour and the
Tests were carried out using an axial loading system, especially designed for the push-out experiences. The hydraulic jack was connected to a load cell and will push-out concrete along the flanges and web of steel profile. At the other extremity another load cell was positioned for
reaction force measurement. Concrete displacement was measured with a wire potentiometer
position sensor (displacement transducer with an accuracy of +/- 0,1 [mm]), connected to an
acquisition data centre.
To control the beating process and to measure temperature inside concrete and over the steel
beam, type K thermocouples were positioned in specific places according to figure 4. An extra
tbennocouple was installed over the external concrete surface to track the heating temperature
delivered by the heating power unit (bulk temperature).
PUSh-Olil tests/or partially encased beams at elevated temperature
+'1-" 0 :-::_
IGII " 1l,' =, + .... r:c ' " , 'E 'J I_
~ ~ ' l ".
" U I. _ _ • . . " . .
--Figure 4 - Thermocouples position for temperature measurement.
3.2 Experimental results
Temperature was incremented inside insulated chamber, using an heating system with 70
[kVA], with electro-ceramic resistances applied to beam flanges. Temperature in steel and concrete follows the prescribed heating curve, as represented in figure 5.
-- PTe l ~ P T C ~ - PTO - p'rr.j ~~ W T SI -- WT S1 - - \\753 ~ \ \"TS · l I ~ O
t· ... · ... , ...
... : ....+; .. ···· .. ·[··· ....
J)? . :
'0 . "
<) ~ O()O ·woo 6000 worm
Figure 5 - Measured temperatures during heating process, for natural adherence.
After temperature stabilization, the mecbanicalloading process began. Concrete did not present any visible crack or crushing failure under axial load. Push-out experiments were conducted with breaking of natural adherence, as represented in figure 6. When adhesion bond breaks, a negative pending appears in load-displacement curve. The final curve behaviour corresponds to friction at interface level between concrete and steel surface.
Paulo A. G. Piloto, Ana B. Ramos Gavilol1 • Luis M R. Mesquita and Luisa Ban'eira
... T1.""51 I < - Tel ll -e-TClt 3
""00,-3: ·10 000
~ 30000 •
R c bU ~c concrete dliplacC"menl (nunJ
Figure 6 - Load-displacement results at elevated temperature with natural adherence.
The maximum shear stress for natural bond adherence was determined for this temperature level for all tests. Differences between results may be justified by the fact that both concrete blocks travel at the same time for test I, while test 2 presented local failure in one block, followed by large concrete displacement. The third test followed measured force displacement of the first test with higher maximum shear stress, but with the same characteristic bebaviour. See table I for maximum bond strength.
Table I - Maximum bond strength results. Tested beam Max. force [NJ Max. Bond stress [MPa]
Test 1 44142 0.293
Test 2 45487 0.302
Test 3 71689 0.476
4. NUMERICAL SIMULATION FOR PUSH-OUT
4.1 Numerical model
Thermal and mechanical non linear analyses were applied to simulate the experimental push-out tests for partially encased beams. Results are presented at elevated temperature, using the experimental bond bebaviour between steel and concrete. A three dimensional finite element model was used to simulate thermal and mechanical analysis, base on Ansys finite element solutions, . One part of the mesh was generated with finite shell elements to represent steel profile and the other mesh with solid and link elements to model reinforced concrete. These meshes were joined by non-linear finite spring elements used to simulate bond behaviour, see figure 7.
Push-out tests Jar partially encased beams at elevated temperature
I , I,
I-- . '- ~'
a) Thennal model. b) Mechanical model.
Figure 7 - Finite Element model for bond analysis.
Thermal model required non linear unsteady solutions for the experiments simulation at
elevated temperatures, using appropriate thermal conductance for the interface between steel and reinforced concrete. An optimum design strategy was conducted to determine the best approach to this interface property, based on the minimization of the squared relative error between numerical temperature results and experimental measured temperature, see Eq. 1.
2:::I ~ p 1
1= 1 1',
This design variable (contact conductance) was estimated by numerical design optimization,
using the first order method. The objective function, error, was considered to minimize differences between predicted and measured temperature values, in space and in time,
according to the previous equation and the specific measured temperature values. The first order method uses gradients of the dependent variables with respect to the design variables.
Gradient calculations are performed in order to detennine a search direction. Each optimization iteration accounts for a number of sub-iterations that includes search direction, gradient
computations and several thermal analyses loops. A conductance value of 100 [W Im' K] was
considered for the interface steel-concrete, being in accordance with reference .
Thermal and mechanical properties were adopted from eurocode, [9,10], to simulate steel and concrete behaviour. An elasto-elliptic-plastic model was adopted for steel, using the appropriate experimental values. Concrete being quasi brittle material was simulated with
different behaviour for tension and compression, as represented en figure 8. Concrete should be able to crack in tension and crush in compression, using appropriate failure criteria developed
by Willarn Warnke, .
Paulo A. G. Piloto, Ana B. Ramos Gavilim, Luis M R. Mesquita and Luisa Barreira
a) Stress - Strain for concrete. b) Stress - Strain for steel. Figure 8 - Mechanical behaviour for materials.
The mechanical model requires material and geometrical non-linear solutions to simulate large
displacement and an incremental displacement method (maximum 0.12 [mmJ). Force was
simulated by means of step incremental displacement, in the concrete nodes of the loading section. This loading condition satisfies numerical convergence, using Newton-Raphson displacement criteria.
The numerical model for reinforcement considered no movement between steel and concrete. Bond behaviour was represented by non linear finite spring elements, used in nonnal and tangential directions. Higher stiffuess was applied to [mite spring elements in nonnal direction to restrain contact between concrete and steel surfaces. Experimental measured stiffness was applied in tangential direction to validate experimental tests. Bond stress behaviour was modelled by finite spring elements with experimental nonlinear generalized force-deflection ability.
4.2 Numerical results
Numerical simulation predicts nodal temperature values as represented in figure 9. Good agreement was achieved between experimental results and numerical simulation.
· 1 ~0
~ 150 100
... " .. ,51-Exp~riltlcmnl
__ WTSI_ Nlllu ericul
WTS3-E)(l~ril!letllnl .... - WT52-E.. ~Jl e rimcntal
- \ \'1:53 -N Uluc ri~n l --\VI S2- Nlltlicrical I
o lUoo :000 300 0 .tom) 5000 6000 700 0 8000
Figure 9 - Comparison between experimental and numerical results for temperature prediction.
Push-out tests for partially encased beams at elevated temperature
Numerical results for the simulation of push-out tests are represented in figure 10. Collapse occurs between steel and concrete surface by adherence failure .
110000 70 000 6UOOO 50000 Z l",U)()(H}
~ 30000 20000 10000
NlU Jeri ' n1 , ,
.... Tot 1
Di s !,l J.~ m c u l (m ]
Figure 10 - Numerical results for push-out test simulation.
A new set-up was developed for push-out experiments at elevated temperature, More experiences were conducted at room temperature with natural adherence and with shear connectors welded to the web of steel profile.
Bond stress and bond behaviour were experimentally determined at elevated temperature for natural adherence. The results show that shear strength on web and flanges is higher than the
expected value from eurocode (TRd~0.2 [MPa]), .
The results at elevated temperature presented a decrease in bond strength relative to room temperature results.
Numerical validation was also presented for this adherence condition, considering the corresponding experimental value for bond behaviour at contact elements. Interface between steel and concrete was numerically modelled by means of non-linear finite spring element, considering appropriate conductance and stiffness as presented.
 Georgali, B.; Tsakiridis, P.E.; "Microstructure of fire-damaged concrete. A case study.";
Cement & Concrete Composites 27, 2005, pp. 255-259.
 ICS, ISO 4287, "Geometrical product specification (GPS)" - surface texture: Profile method - terms, definitions, and surface texture parameters, Switzerland, 1997.
Paulo A. G. Piloto, Ana B. Ramos Gavilcin , Luis M R. Mesquita and Luisa Ban'eira
[3) ICS, ISO 4288, "Geometrical product specification (GPS)" - surface texture: Profile method - rules and procedures for the assessment of surface texture, Switzerland, 1996.
 Silva, Romulo Danilli, "Estudo da aderencia a,o concreto em pilares mistos preenchidos" (in portuguese); Master of Science Thesis; Sao Jorge School of Engineering, Silo Paulo, Brazil, March 2006.
[5) NP EN 10002-1 , "Metallic materials. Tensile testing. Part I: Method oftest (at ambient temperature)"; 1990.
[6) NP EN 12390 - 3, "Testing hardened concrete. Part 3: Compressive strength of test specimens", 2003.
[7) Ansys INC; "ANSYS Academic version", Release 10.0, Help System, 2006.
[8) Ghojel, J, Experimental and analytical technique for estimating interface thermal
conductance in composite structural elements under simulated fire conditions,
Experimental Thermal and Fluid Science, No. 28, 2004, pp. 347-354.
[9) CEN; EN 199312; Eurocode 3, Design of steel structures Part 12: General rules -Structural fire design, April 2005.
[10) CEN; EN 1992-1-2, "Eurocode 2: Design of concrete structures - Part 1-2: General rules-Structural fire design"; December 2004.
[11) CEN - EN 1994-1-1 ; "Eurocode 4: Design of composite steel and concrete structures-Part I-I: General rules and rules for buildings"; Brussels, December 2004.